The Southern African Institute of Mining and Metallurgy Furnace Tapping Conference 2014 D.J. Rioux, T.A. Moore, G.J. McTeer, and D.L. Verhelst
Tecks KIVCETTM lead tapping experience
D.J. Rioux, T.A. Moore, G.J. McTeer, and D.L. Verhelst Teck Metals Ltd
Teck Metals Ltd operates an integrated zinc-lead complex at Trail, British Columbia, Canada. Since 1997, KIVCETTM flash smelting technology has been utilized for the treatment of zinc plant residues and lead concentrates. Trail Operations furnace uses four water-cooled jackets for bullion tapping. This paper provides an overview of KIVCET bullion tapping for the past 16 years, and discusses successes and challenges encountered with respect to operations, training, and monitoring.
Teck Metals Ltd has operated an integrated zinc-lead complex at Trail, British Columbia since the early 1900s. Close integration between the zinc and lead operations is key to maximizing metal recovery and ensuring the financial success of Trail Operations. A major advantage of this site is the ability of the lead smelting operations to treat all zinc plant iron residues currently produced, as well as stockpiled iron residues that were produced prior to the smelter modernization in 1997 (Ashman et al., 2000; Goosen and Martin, 2000).
The smelter modernization consisted of a new KIVCETTM furnace along with a new state-of-the-art slag fuming furnace and a new drossing plant.
The heart of the lead smelting process is the KIVCET furnace shown in Figure 1 (Rioux et al., 2008) The KIVCET
furnace treats a dried mixture of lead concentrates, coal fuel, silica and limestone fluxes, plant recycles, and Zn plant residues mixed with a small amount of coke, and recycle dust coming from the waste heat boiler and electrostatic precipitator. The feed mixture ignites in the reaction shaft to reach a temperature of about 1425C, desulphurizing the smelt through sulphide combustion and sulphate decomposition. The coke is sized to minimize oxidation so that it accumulates on the molten bath to form a coke checker where lead oxide formed in the reaction shaft is reduced to lead bullion and some ferric iron is reduced to ferrous. Lead bullion and molten slag exit the coke checker and travel under a water-cooled partition wall to enter the electric furnace.
Figure 1. Schematic Diagram of the KIVCET furnace and ancillary equipment
Furnace Tapping Conference 2014
The two primary functions of the electric furnace are phase disengagement and settling of the molten slag/bullion mixture, and heat transfer under the partition wall to complete the heat balance for the endothermic reduction reactions in the coke checker.
The engineering solutions used for the KIVCET furnace were developed and selected to provide excellent furnace integrity given the process requirements of containing molten lead bullion and an aggressive slag.
The furnace consists of large water-cooled copper elements bolted together to form the furnace sidewalls that contain the slag and the upper levels of the lead bullion. Some of the copper elements incorporate tap-holes for the slag and lead bullion. The walls of the reaction shaft, and some of the uptake shaft before the transition to the waste heat boiler, are also constructed of large water-cooled copper elements. A forced-convection air-cooled refractory hearth contains the lead bullion. The hearth construction consists of two layers separate by a thin stainless steel sheet. The purpose of the steel sheet is to prevent lead penetration below the working lining and also to allow for slippage between the two layers. The working lining is a chrome-magnesite brick to provide chemical resistance and the bottom layer is a highly conductive carbon brick to enhance the cooling of the working lining. The upper sidewalls above the copper castings of the electric furnace portion, as well as the arch in this section, are constructed of chrome-magnesite refractories. The arch design is a combination of a sprung construction with a secondary brick suspension system to ensure a gas-tight design.
Lead is removed from the furnace at intervals of approximately 2.5 hours via one of four tap-holes located on the side of the furnace, while slag is removed via one of two tap-holes located at the end of the furnace, as shown in Figure 1. The bullion and the slag operating temperature contain significant levels of superheat up to 800C and 150C, respectively. For the Trail furnace, the design of the lead bullion tap-hole in particular is unique because of the need to remove bullion from the side of the furnace, compared to the siphon design, which is located at the end of the furnace in other similar furnaces. Effective training and operational and monitoring practices are needed to allow for reliable tapping of the lead bullion.
The lead tap-hole is made up of two cast copper parts: the tapping jacket and the tapping insert. The jacket is part of the furnace wall construction and can be replaced during major furnace shutdowns when the furnace has been drained. The insert is a small casting which can be changed without draining the furnace. Figure 2 is a schematic representation of the jacket and insert configuration. Both castings are made with water cooling channels and equipped with temperature sensors.
Figure 2. Cross-sectional representation of the lead tapping channel
The upper section of the water-cooled copper tapping jacket is partially lined with a chrome-magnesite refractory and
a castable refractory is installed on the lower section around the tapping channel. Two water circuits ensure adequate cooling of the element during tapping operations.
Tecks KIVCETTM lead tapping experience
The tapping channel is made up of two parts. The first part is a silicon carbide refractory cone brick at the front of the tapping channel with the cooled copper insert behind it. A silicon carbide sleeve is installed in the copper insert to protect the copper during tapping.
A manually operated hydraulic mudgun is used to close the tap-hole. The tapping operator uses a drill attached to the mudgun to open the hole. At times it may be necessary for the operator to use an oxygen lance to open the hole if drilling is unsuccessful. The oxygen lance is also used to clear out any buildup material in the tapping channel to ensure the drill is properly directed down the channel. Misdirection of the drill bit will cause mechanical damage to the silicon carbide components.
It is very important that the furnace operator closely assesses the condition of the tapping channel components. In addition to visual inspections of wear, the operating conditions of the castings are monitored to assess the state of the system at any given time. The instrumentation monitors copper temperatures, water temperatures, and water flow rates.
Each set of tapping jackets is equipped with 13 thermowells for monitoring of temperatures at different copper locations. The majority of the thermowell locations are around the throat of the jacket where the Pb bullion flows, as seen in Figure 3.
Figure 3. Thermowell locations on KIVCET lead tapping jackets
A closed-circuit water system is used to cool the copper castings, and the temperature of the water entering the
casting is maintained at 40C. Water flows and outlet water temperature are recorded by resistance temperature detectors (RTDs) for all three circuits (primary, secondary, and insert). All instrument data is fed to a central control room which is staffed 24/7 so that any alarms can be reacted to immediately. The cooling circuit for cast copper inserts is designed to maintain the insert below 50C during lead tapping. The operating temperature of the insert, as well as the temperature rise of the cooling water as it passes through the insert, are closely monitored. The furnace operator will take corrective measures should the temperature of the insert exceed 70C or the cooling water temperature differential increase more than 10C. Either change could be a result of a decrease in the cooling capacity of the insert or a deterioration of the protective silicon carbide sleeve installed in the insert. Following an alarm, a review of the tap-hole performance by plant technical personnel, including an insert silicon carbide sleeve inspection, is completed before the tap-hole is put back into operation.
In addition, the instrument readings are fed into a bullion tapping guidance system (BTGS) that was developed by Hatch in 2004 (Plikas et al., 2005). It consists of a computational fluid dynamics (CFD) model that relates thermocouple readings, bullion temperatures, and increases in water temperatures to jacket conditions and coil bonding. It then uses multivariate statistical analysis (principal component analysis) to monitor each tap in real time to identify unusual conditions. When a tapping anomaly is identified, an e-mail is sent out to Tecks furnace specialists for review. The original intent of the system was to have the results sent directly to the operators but this was not implemented, due mainly to many false positives. The overall results have been used to give a qualitative representation of refractory wear in the front of the tapping jackets, along with an indication of when this wear occurs, as seen in Figure 4.
Furnace Tapping Conference 2014
Figure 4. BTGS-predicted minimum thickness for a bullion tapping jacket (20102013)
Operational and maintenance history
When the KIVCET furnace began operation in March 1997 there were three lead tapping jackets with copper inserts. One additional tapping jacket that did not contain an insert